Controlling multiple orderings in metal thiocyanate molecular perovskites Ax{Ni[Bi(SCN)6]}
Lee, Jie Yie; Ling, Sanliang; Argent, Stephen P.; Senn, Mark S.; Cañadillas-Delgado, Laura; Cliffe, Matthew J.; Chemical Science 12 (2021) 3516–3525; doi:10.1039/D0SC06619B

data_1560103
_publ_section_title
;
 Controlling multiple orderings in metal thiocyanate molecular perovskites
 Ax{Ni[Bi(SCN)6]}
;
_journal_issue                   10
_journal_name_full               'Chemical Science'
_journal_page_first              3516
_journal_page_last               3525
_journal_paper_doi               10.1039/D0SC06619B
_journal_volume                  12
_journal_year                    2021
_chemical_formula_moiety         'Bi0.667 C4 N4 Ni0.667 S4, 0.667(H4 N)'
_chemical_formula_sum            'C4 H2.67 Bi0.67 N4.67 Ni0.67 S4'
_chemical_formula_weight         422.81
_chemical_name_systematic        'Ammonium nickel hexathiocyanatobismuthate'
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   difmap
_audit_creation_date             2020-04-29
_audit_creation_method
;
Olex2 1.3
(compiled 2020.01.31 svn.r88ba2a32 for OlexSys, GUI svn.r6032)
;
_audit_update_record
;
2020-11-18 deposited with the CCDC.	2021-01-15 downloaded from the CCDC.
;
_cell_angle_alpha                97.5740(10)
_cell_angle_beta                 92.1370(10)
_cell_angle_gamma                91.8170(10)
_cell_formula_units_Z            3
_cell_length_a                   8.44100(10)
_cell_length_b                   8.68990(10)
_cell_length_c                   11.8177(2)
_cell_measurement_reflns_used    9374
_cell_measurement_temperature    20(2)
_cell_measurement_theta_max      60.791
_cell_measurement_theta_min      4.585
_cell_volume                     858.10(2)
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_diffrn_ambient_temperature      20(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.848
_diffrn_measurement_device_type  'D19, Institut Laue Langevin'
_diffrn_radiation_type           neutrons
_diffrn_radiation_wavelength     0.94558
_diffrn_reflns_av_R_equivalents  0.0311
_diffrn_reflns_av_unetI/netI     0.0236
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.848
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            18745
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.848
_diffrn_reflns_theta_full        34.566
_diffrn_reflns_theta_max         60.791
_diffrn_reflns_theta_min         4.585
_exptl_absorpt_coefficient_mu    0.04734
_exptl_absorpt_correction_T_max  0.9203
_exptl_absorpt_correction_T_min  0.8824
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            'dark orange'
_exptl_crystal_colour_modifier   dark
_exptl_crystal_colour_primary    orange
_exptl_crystal_density_diffrn    2.455
_exptl_crystal_description       block
_exptl_crystal_F_000             592
_exptl_crystal_recrystallization_method
'Re-crystallisation from solvent: butanone'
_exptl_crystal_size_max          2.9
_exptl_crystal_size_mid          2.5
_exptl_crystal_size_min          2.2
_refine_diff_density_max         1.227
_refine_diff_density_min         -1.752
_refine_diff_density_rms         0.251
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.151
_refine_ls_hydrogen_treatment    refall
_refine_ls_matrix_type           full
_refine_ls_number_parameters     232
_refine_ls_number_reflns         9590
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.151
_refine_ls_R_factor_all          0.0460
_refine_ls_R_factor_gt           0.0448
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0394P)^2^+6.1942P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1111
_refine_ls_wR_factor_ref         0.1117
_reflns_Friedel_coverage         0.000
_reflns_number_gt                9374
_reflns_number_total             9590
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d0sc06619b3.cif
_cod_data_source_block           1NH4NiBiSCN6_20K_neutron
_cod_depositor_comments
'Adding full bibliography for 1560103--1560109.cif.'
_cod_database_code               1560103
_shelx_shelxl_version_number     2018/3
_olex2_refinement_description
;
;
_shelx_res_checksum              88588
_olex2_submission_special_instructions 'No special instructions were received'